Biomechanical Behavior of Extensively Restored Premolars: Cusp Deformation, Marginal Integrity, and Fracture Resistance Bruno de Castro Ferreira Barretoa / Bart Van Meerbeekb / Annelies Van Endec / Silas Junior Boaventura de Sousad / Gisele Rodrigues da Silvae / Paulo Vinícius Soaresf / Carlos José Soaresg
Purpose: To study the biomechanical behavior of extensively restored premolars by determining the effect of the composite type, presence of cusp weakening, and compressive loading on the cusp deformation (CD), marginal integrity (MI), and fracture resistance (FR) of directly restored premolars. Materials and Methods: Forty premolars received Class II mesio-occlusal-distal (MOD) cavities and were divided into 4 groups (n = 10) in accordance with the two study variables: composite type (conventional: Filtek Z250 XT [Z250], 3M ESPE; low shrinkage: Venus Diamond [VD], Heraeus-Kulzer) and the presence of cusp weakening (with/without). Cusp deformation upon restoration was assessed using strain gauges during the restorative procedure and thereafter when the restorations were subjected to an occlusal load of 100 N. The samples were subjected to thermal and mechanical cycling. Epoxy resin replicas of the proximal tooth/restoration interfaces were made to analyze the marginal integrity (MI) using scanning electron microscopy. To determine the fracture resistance (FR), the teeth were loaded at a crosshead speed of 0.5 mm/min until fracture. Results: The conventional composite Z250 had higher CD, lower MI, and lower FR than the low-shrinkage composite VD. Cusp weakening had no influence on CD, but MI and FR decreased. Conclusion: The low-shrinkage composite VD performed better in restoring extensively destroyed premolars than did Z250. Keywords: composite, premolar, shrinkage stress, cusp deformation, marginal integrity, fracture resistance. J Adhes Dent 2015; 17: 213–218. doi: 10.3290/j.jad.a34136
Submitted for publication: 27.09.14; accepted for publication: 15.04.15
he choice of the most suitable material to restore large cavities in posterior teeth still generates doubt among clinicians, particularly when the cusps are weakened. Direct composite restorations are placed mostly
thanks to their favorable physical, mechanical, and esthetic characteristics.9 These materials have an elastic modulus (E) similar to that of dentin and can be bonded to dental substrates. They can mimic the biomechan-
Research Fellow of Biomechanics Research Group, Department of Restorative Dentistry and Dental Materials, School of Dentistry, Federal University of Uberlândia, Uberlândia, Minas Gerais, Brazil. Performed the experiments, wrote the manuscript.
Professor, Biomechanics Research Group, Department of Restorative Dentistry and Dental Materials, School of Dentistry, Federal University of Uberlândia, Uberlândia, Minas Gerais, Brazil. Contributed substantially to the thermal and mechanical cycling tests.
Professor and Chairman, KU Leuven – BIOMAT, Department of Oral Health Sciences, Conservative Dentistry, University Hospitals Leuven, Leuven, Belgium. Reviewed the manuscript, contributed substantially to the discussion.
PhD Student, KU Leuven – BIOMAT, Department of Oral Health Sciences, Conservative Dentistry, University Hospitals Leuven, Leuven, Belgium. Reviewed the English language, proofread the manuscript, contributed substantially to the discussion.
Professor, Biomechanics Research Group, Department of Restorative Dentistry and Dental Materials, School of Dentistry, Federal University of Uberlândia, Uberlândia, Minas Gerais, Brazil. Contributed substantially to experimental design.
Professor and Chairman, Biomechanics Research Group, Department of Restorative Dentistry and Dental Materials, School of Dentistry, Federal University of Uberlândia, Uberlândia, Minas Gerais, Brazil. Idea, hypothesis, reviewed the manuscript.
Research Fellow, Biomechanics Research Group, Department of Restorative Dentistry and Dental Materials, School of Dentistry, Federal University of Uberlândia, Uberlândia, Minas Gerais, Brazil. Contributed substantially to the strain-gauge tests.
Vol 17, No 3, 2015
Correspondence: Dr. Carlos José Soares, Operative Dentistry and Dental Materials area, School of Dentistry, Federal University of Uberlândia UFU, R: Republica do Piratini S/N Bloco 4LA, Campus Umuarama, Bloco 4L-A, sala 4L-A42, Uberlândia, MG, Brazil 38405-902. Tel: +55-34-3218-2255, Fax: +55-34-3218-2279. e-mail: [email protected]
Barreto et al
ical behavior of unrestored teeth, thereby improving the overall strength of the tooth-restoration biomechanical unit.18-20 Composite restorations can reduce the occurrence of fractures of partially destroyed teeth, primarily in maxillary premolars, which due to their anatomy present an elevated rate of catastrophic failures.8 The polymerization shrinkage inherent in dental composites generates stress within the restored tooth, especially at the tooth/composite interface.3,4,15 Shrinkage stress has been associated with cusp deformation, loss of marginal integrity, crack propagation, microleakage, and postoperative sensitivity.24 Shrinkage stress is not a material property, but depends on the combination of many factors, such as composite material characteristics, restoration geometry, and restorative technique.14,18,19 When collective stress from polymerization shrinkage and occlusal chewing forces exceeds the maximum stress the tooth-restoration complex can endure, it must contribute to the fracture of the tooth-restoration complex, although the current literature is not clear on the effect of the association of stresses generated by polymerization shrinkage and chewing forces.1,2 Dimethacrylates, such as bis-GMA (bisphenol-A glycidyl methacrylate), have been the most commonly used monomers in dentistry for more than 50 years.6 Diluent co-monomers, such as TEG-DMA (triethyleneglycol dimethacrylate), are added in order to reduce the paste viscosity, but they increase the volumetric shrinkage.10 In order to minimize polymerization shrinkage and its undesirable effects, novel low-shrinking monomers, such as TCD urethane (tricyclodecane-urethane dimethacrylate), have been synthesized.5 This monomer consists of three ring structures connected in the center of a backbone, making the polymer more flexible and thus helping to control shrinkage, yet not increasing the viscosity and therefore reducing the need for diluents.5 However, studies on the performance of this new composite with respect to its biomechanical behavior in the tooth-restoration unit are lacking to date. Since shrinkage stress cannot be measured directly,23 only laboratory tests can demonstrate its effects.24 A destructive mechanical test used to determine fracture resistance enables the analysis of tooth behavior in situations of high-intensity loading.18 However, this test has limitations with regard to obtaining information on the internal behavior of the tooth-restoration complex.18 Therefore, the addition of an experimental nondestructive method, such as strain gauges, is highly desirable. Strains caused by cusp deformation can be recorded with strain gauges, which use electrical conductors that can be adhered to external tooth surfaces to record the local strains on deformed cusp surfaces during polymerization.14 Another nondestructive method involves the use of epoxy resin replicas to semi-quantitatively evaluate the marginal integrity using scanning electron microscopy (SEM).7 Therefore, the aim of this study was to examine the biomechanical behavior of extensively restored premolars by determining the effect of the composite type, as well as the presence of cusp weakening and compressive loading on the cusp deformation (CD), marginal integrity (MI), and fracture resistance (FR) of directly restored premolars. The null hy214
pothesis was that neither the composite type, the presence of cusp weakening, nor the compressive loading have an influence on the CD, MI, and FR of the restored premolars.
MATERIALS AND METHODS Preparation of Samples Forty sound human maxillary premolars with similar crown size and shape were selected (approved by the Ethics Committee of Piracicaba Dental School, UNICAMP, #168/2009) and stored in 0.5% aqueous chloramine solution at 4°C for a maximum of 3 months. The teeth were selected to have an intercuspal width within a maximum deviation of not more than 10% of the determined mean. The measured intercuspal width ranged from 6.5 to 7.9 mm. The teeth were embedded in polystyrene resin (Cristal; Piracicaba, SP, Brazil) up to 2 mm below the cementoenamel junction to simulate the alveolar bone. Periodontal ligaments were simulated inside the cylinder using a polyether impression material (Impregum F, 3M ESPE; St Paul, MN, USA) following the protocol of Soares et al.17 Mesial-occlusal-distal (MOD) Class II cavities were cut using a standard preparation machine16 equipped with a cylindrical diamond bur (#3099, KG Sorensen; Cotia, SP, Brazil). The width of the cavity was determined as 3/4 of the intercuspal distance; the occlusal preparation was 2 mm deep and the proximal boxes were 3.5 mm deep. The prepared teeth were divided into 4 groups (n = 10) according to combinations of the two study factors: the composite used (conventional composite Filtek Z250XT [Z250], shade A2, 3M ESPE, vs low-shrinkage composite Venus Diamond [VD], shade A2, Heraeus Kulzer; Hanau, Germany) and the cavity conditions (sound cusps [S], or weakened cusps [W]). In group W, the buccal and lingual cusps were both undermined using a pear-shaped diamond bur (#3168, KG Sorensen), resulting in an undercut with a width of approximately 1.2 mm (Fig 1a). Cusp Deformation Measurement Cusp deformation was measured with strain gauges (PA 125AA-120Ω, Excel Sensores; São Paulo, Brazil), which had an internal electrical resistance of 350 Ω, a gauge factor of 2.07, and a grid size of 10.11 mm2. The gauge factor is a proportional constant between the electrical resistance variation and strain. The strain gauges were bonded to the cervical area of the buccal and lingual surfaces with cyanoacrylate glue (Super Bonder, Loctite; São Paulo, Brazil), and the wires were connected to a data acquisition device (ADS0500IP, Lynx Tecnologia Eletrônica; São Paulo, SP, Brazil) equipped with the data analysis software AqDados 7.02 and AqAnalisys (Lynx Tecnologia Eletrônica). Strain gauges were placed at the middle area of the enamel cusps. In addition, two strain gauges were fixed to another intact tooth to compensate for dimensional deviations due to temperature effects. The teeth were restored following the manufacturer’s recommendations, using a two-step etch-and-rinse adhesive (Single Bond, 3M ESPE) in all groups. A Teflon matrix The Journal of Adhesive Dentistry
Barreto et al
S N = 20
W N = 20
N = 40
a Fig 1 Set-up of experiment. (a) Preparation of sample. (b) Cusp deformation measurement. (c) Thermal and mechanical cycling. (d) Marginal integrity examination. (e) Fracture resistance. Abbreviations: S, sound cusps; W, weakened cusps; Z250, conventional composite Filtek Z250XT; VD, low-shrinkage composite Venus Diamond.
F = 100N
Z250 N = 10 VD N = 10 Z250 N = 10
Buccal strain gauge
Buccal strain gauge
Lingual strain gauge
Lingual strain gauge
Preparation of samples
5°C 37°C ImageJ
Thermal and mechanical cycling
encompassing a cylindrical space of 13.8 mm3 was used to standardize the volume of each composite increment before insertion into the cavity. The teeth in the S group were restored in eight increments and the ones in the W group in ten increments using an oblique layering technique. Each increment was cured for 40 s using a halogen light source with an output of 600 mW/cm2 (Optilux 500, Demetron, Kerr; Orange, CA, USA), which was measured with the light meter that was part of the light curing unit. The total energy output for each restoration was 192 J/ cm2 in the S group and 240 J/cm2 in the W group. The strain values were recorded at a frequency of 4 Hz during the restorative procedure and the recording was continued for 10 min after curing the last increment. Next, the specimens were submitted to compressive loading applied with an 8 mm sphere which contacted the tooth structure solely at the ridges of buccal and lingual cusps at a speed of 0.5 mm/min, up to a maximum of 100 N in a mechanical testing machine (EMIC DL 2000, EMIC Equipamentos e Sistemas de Ensaio; São José dos Pinhais, PR, Brazil) (Fig 1b). The strain measurement results of each group were submitted to statistical analysis using 3-way ANOVA and Tukey’s test (α = 0.05), considering the additional factor compressive loading (with/without), for buccal and lingual cusps independently. Thermal and Mechanical Cycling After the cusp-deformation measurement, the samples were finished with fine diamond burs (#2135FF, KG Sorensen) at low speed under water spray and polished with Sof-Lex disks (3M ESPE). The teeth were then submitted to 6000 thermal cycles using a thermocycling machine (Thermal Cycler ER- 26000, ERIOS Equipamentos; São Paulo, SP, Brazil).11,22 Thermocycling was performed in Vol 17, No 3, 2015
VD N = 10
bath temperatures of 5°C, 37°C, and 55°C. The dwell time was 30 s and the transfer time 10 s, resulting in 2 min for each cycle. Afterwards, the samples were submitted to 300,000 mechanical loading cycles at a frequency of 4 Hz (LRP 3000, Mechanical loading cycle device, ERIOS Equipamentos) with a vertical load of 50 N. The samples remained in distilled water at 37°C during the whole mechanical cycling process (Fig 1c). Marginal Integrity Impressions of the restorations were next taken using a polyvinyl siloxane impression material (Aquasil Ultra LV, Dentsply; Konstanz, Germany) and replicas of the proximal mesial and distal boxes were made using epoxy resin (Epoxide, Buehler; Lake Bluff, IL, USA). The replicas were mounted on aluminum stubs, gold sputter coated (Leica EM, SCD050, Leica; Wetzlar, Germany), and examined with SEM (EVO NA 10, Carl Zeiss; Jena, Germany) (Fig 1d). The adhesive margins were divided into nine regions per surface (Fig 2a) and analyzed at 200X magnification. Each region was classified as gap, continuous margins, or artifact (Figs 2b to 2d); the result was semiquantitatively classified per region and expressed as a percentage using Image J Software (public domain, Javabased image processing and analysis software, National Institutes of Health; Bethesda, MD, USA). Fracture Resistance Afterwards, the specimens were submitted to compressive loading in a mechanical testing machine (EMIC DL 2000) using an 8-mm diameter metal sphere at a crosshead speed of 0.5 mm/min until fracture (Fig 1e). The results were statistically analyzed with two-way ANOVA and Tukey’s test (α = 0.05). 215
Barreto et al 4
Artifact Continuous margins
RESULTS Cusp deformation for the two composites (Z250, VD), the two cavity preparation conditions (with/without cusp weakening), and the two loading conditions (with/without compressive loading) are shown in Tables 1 and 2 for the buccal and lingual cups, respectively. Results of testing for interaction effects between groups are shown in Tables 3 and 4. Cusp weakening only influenced the buccal cusp deformation when the composite VD was used and the teeth were not loaded. The low-shrinkage composite VD resulted in significantly lower CD than did the conventional composite Z250, except on buccal cusps when the specimens were compressively loaded. Compressive loading decreased CD significantly for all groups. The results of the SEM semi-quantitative marginal analyses are shown in Fig 3. Clear gaps were recorded when the cusps were weakened, irrespective of the composite used. The fracture resistance is shown in Table 5 for the four experimental groups. Weakening of the cusps significantly decreased the fracture resistance, irrespective of the composite used (p < 0.05). A significantly higher fracture resistance was recorded for the teeth with the low-shrinkage composite VD than for those restored with the conventional composite Z250 (p < 0.05).
DISCUSSION All study variables – namely, the composite type, cusp weakening, and compressive loading – influenced the biomechanical performance of premolars extensively restored with composite; hence, the null hypothesis was rejected. Cusp deformation, measured using strain gauges, was influenced by composite type, yielding higher values for the conventional composite Z250 than 216
Fig 2 (a) Examples of marginal integrity (MI) in the 9 regions subjected to semiquantitative marginal analysis (%). (b) MI recorded as gap; (c) MI recorded as continuous margins; (d) MI recorded as artifact.
for the low-shrinkage composite VD (Tables 1 and 2). The conventional composite Filtek Z250 XT contains bisGMA monomers with high molecular-weight oligomers.21 Due to its high viscosity, bis-GMA requires the addition of diluent co-monomers, such as bis-EMA (bisphenol A polyethylene glycol diether dimethacrylate), that result in an increase in volumetric shrinkage.10 The lowshrinkage composite Venus Diamond (Heraeus Kulzer), on the other hand, contains the novel tricyclodecane (TCD) monomer TCD-DI-HEA, bis-(acryloyloxymethyl) tricyclo[5.2.1.02.6]decane),12 which is the basis of the new TCD-urethane cross-linking technology. This avoids the need for bis-GMA and short diluent cross linkers, thereby reducing shrinkage and its consequent stress.5 The low-shrinkage composite VD suggested better marginal integrity than did the conventional composite Z250 (Fig 3). This is possibly attributed to the higher shrinkage stress imposed by Z250 than by VD. This shrinkage stress may have compromised the early marginal integrity during the restorative procedure. The conventional composite Z250 resulted in a lower fracture resistance of the premolars than did VD (Table 5). This fact may be due the differences in material properties, for instance, the elastic modulus and post-gel volumetric shrinkage. The resin Filtek Z250 XT has a higher elastic modulus and post-gel volumetric shrinkage than does Venus Diamond.5 This fact might have created wider, deeper marginal gaps for Z250 groups; these gaps could be prone to crack initiation by fatigue and subsequent crack growth by coalescence of microscopic defects evolving into macroscopic defects under the continuous mechanical loading. The type of composite plays an important role in the stress distribution within the tooth-restoration complex. Shrinkage stress is closely related to the volumetric shrinkage of composites, since the former only occurs in the presence of the latter.23 Based on the findings of this The Journal of Adhesive Dentistry
Barreto et al
Table 1 Means and standard deviations of cusp deformation (μS) for the variables composite type, cusp weakening, and compressive loading in buccal cusps Composite type
Weakened cusps (W)
Sound cusps (S)
Filtek Z250 XT (Z250)
Venus Diamond (VD)
Table 2 Means and standard deviations of cusp deformation (μS) for the variables composite type, cusp weakening, and compressive loading in lingual cusps Composite type
Weakened cusps (W)
Sound cusps (S)
Filtek Z250 XT (Z250)
Venus Diamond (VD)
μS: microstrain. Different superscript capital letters represent statistically significant differences for compressive loading in rows and different superscript lower-case letters significant differences for composite type in columns. *Comparison for cusp weakening for the same compressive loading status. Tukey’s test (p < 0.05).
μS: microstrain. Different superscript capital letters represent statistically significant differences for compressive loading in rows and different superscript lower-case letters significant differences for composite type in columns. Tukey’s test (p < 0.05).
Table 3 Results of testing for interaction effects between groups using 3-way ANOVA and Tukey’s test (α = 0.05) for the buccal cusp
Table 4 Results of testing for interaction effects between groups using 3-way ANOVA and Tukey’s test (α = 0.05) for the lingual cusp
Pr > F